Materials and Structures. Indian Institute of Technology Kanpur


 Chad Maxwell
 7 months ago
 Views:
Transcription
1 Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur
2 Lecture 16 Behavior of Unidirectional Composites
3 Lecture Overview Mt Material ilaxes in unidirectional composites Constituent volume fraction and its relationship with composite density Importance of predictive methodologies used for composite material properties Predictive model for longitudinal stiffness Predictive model for longitudinal strength
4 The Need for Predictive Models for Determining Composite Properties Mechanical properties p of a composite material depend on: Properties of constituent materials Orientations of each layer Vl Volume fractions of each constituent t Thickness of each layer Nature of bonding between adjacent layers These properties may be determined by conducting suitable experiments as per industry standards. However, a specific set of experiments can only inform us about a specific fiber matrix system. Hence, if we want to design a composite system by tuning its volume fraction, or fiber matrix combination, or orientation, then a very large number of experiments may have to be conducted.
5 The Need for Predictive Models for Determining Composite Properties Such a process for material property p determination is extremely tedious, prohibitively expensive, and time consuming. Still further, exact fiber matrix i combinations i may not be always available for testing. Hence, there is a need for developing mathematical models, which can reliably predict different thermo mechanical properties of composite materials. Such approaches are very useful for engineers since they provide pp y g y p significant savings in time and cost.
6 Predicting Longitudinal Modulus of Unidirectional Lamina Consider a unidirectional composite lamina with fibers which are continuous, uniform in geometric and mechanical properties, and mutually parallel throughout the length of the lamina. We also assume that the bonding between fiber and matrix is perfect, and thus strains experienced by fb fiber (ε f ), matrix (ε f ) and composite (ε c )are same in longitudinal direction (1 direction). For such a composite, when loaded in 1 direction, the total external load P c will be shared partly by fibers, P f, and partly by matrix, P m. This is shown in Fig Fig. 16.1: Loads on Composite, Fibers, & in a Unidirectional Lamina.
7 Predicting Longitudinal Modulus Unidirectional Lamina We further assume that t fibers and matrix ti bh behave elastically. ll Thus, the expression for stress in fibers, and matrix can be written in terms of their moduli (E f, and E m ) and strains as: σ f = E f ε f and σ m = E m ε m Further, if total cross sectional areas of fibers and matrix are A f and A m m, respectively, then: P f = A f σ f = A f E f ε f, and P m = A m σ m = A m E m
8 Predicting Longitudinal Modulus Unidirectional Lamina Further, we know that load on composite, P c, is sum of P f and P m. Thus, P c = A c σ c = A f σ f + A m σ m, or σ c = (A f /A c )σ f + (A m /A c )σ m However, for a unidirectional composite, A f /A c and A m /A c are volume fractions for fiber and matrix, respectively. Hence, σ c = V f σ f + V m σ m = (V f E f + V m E m ) ε (Eq. 16.2) And, if Eq. 4.2 is differentiated with respect to strain (which is same in fiber and matrix) then. dσ c /dε = V f (dσ f /dε)+ V m (dσ m /dε), or E c = V f E f + V m E m (Eq. 16.3)
9 Predicting Longitudinal Modulus of Unidirectional Lamina Equations 16.2 and 16.3 show that contributions of fibers and matrix to average composite tensile modulus and stress are proportionately t dependent on their respective volume fractions. In general, matrix material has a nonlinear stress strain response curve. For unidirectional composites having such nonlinear matrix materials, Eq works well in terms of predicting their stress strain. strain However, the stressstrain response curve in such materials may not show up as strongly nonlinear, since fibers, especially when their volume fractions are high, dominate their stress strain t response. The higher the fiber volume fraction, the closer is the stress strain curve for The higher the fiber volume fraction, the closer is the stress strain curve for a unidirectional lamina to that for the fiber.
10 Predicting Longitudinal Modulus of Unidirectional Lamina Experimental data pertaining to tensile test specimens of lamina agree very well with Eqs and However, the results for compressive tests are not all that agreeable. This is because fibers under compression tend to buckle, and this tendency is resisted by matrix material. This is analogous to a structure with several columns on an elastic foundation. For a unidirectional composite, the compressive response is strongly dependent on shear stiffness of matrix material. Further, Eq shows us that load shared by fibers may be increased either by increasing fiber stiffness or by increasing its volume fraction. However, experimental data show that it becomes impractical to aim for fiber volume fractions in excess of 80% due to issues of poor fiber wetting and insufficient matrix impregnation between fibers.
11 Predicting Longitudinal Strength of Unidirectional Lamina To predict longitudinal strength of a unidirectional ply, requires one to understand the nature of deformation of such a ply as load increases. In general, the stress strainstrain response of unidirectional plies under tension undergoes four stages of change. In first stage, when stresses are small, fiber as well as matrix materials exhibit elastic behavior. Subsequently, matrix starts becoming plastic, while most of the fibers continue to extend elastically. In the third stage, both hfb fibers and matrix deform df plastically. ll This may not happen in case of glass or graphite fibers, as they are brittle in nature. Finally, the fibers fracture leading to sudden rise in matrix stress, which in turn leads to overall composite failure. A unidirectional lamina starts to fail in tension, whenits fibers are stretched to their ultimate fracture strain. Here it is assumed that all of its fiber fail at the same strain level. If at this stage, the volume fraction of matrix is below a certain threshold, the it will not be able to absorb extra stresses transferred to it due to breaking of fibers. In such a scenario, the entire composite lamina will fail.
12 Predicting Longitudinal Strength of Unidirectional Lamina Thus, ultimate tensile strength of a unidirectional ply can be calculated as: σ uc = V f σ uf + (1 V f )σ m (Eq. 16.4) where σ uc and σ uf are ultimate tensile strengths of ply and fiber, respectively, and σ m is stress in matrix at a strain level equaling fracture strain in fiber. If the fiber volume fraction does not exceed a certain threshold (V min ), then even if all the fibers break, the matrix the total load on the composite. In such a condition, the ultimate tensile strength of composite may be written as: σ uc = V m σ um = (1 V f )σ um (Eq. 16.5) The relation for V min, can be developed dby equating Eqs and 16.5, replacing V f by V min, and solving for the latter. This is shown in Eq V min = (σ um σ m )/(σ uf + σ um σ m ) (Eq. 16.6)
13 Predicting Longitudinal Strength of Unidirectional Lamina Further, a well designed unidirectional lamina requires that its ultimate tensile strength should exceed that of matrix. This can happen only when; σ uc = V f σ uf + (1 V f )σ m σ um, where σ um is ultimate tensile strength of matrix. This equation is satisfied only if fiber volume fraction exceeds a certain critical value, which is defined as: V crit = (σ um σ m )/(σ uf σ m ) (Eq. 16.7) Thus, if: V f < V min, then failure of matrix will coincide with failure of composite, while fibers will fail prior to failure of matrix. V f = V min, then failure of matrix, fiber and composite will happen at the same time. V f > V min, then failure of fiber, will immediately lead to failure of matrix as well as of the composite. V f > V crit, then failure of fiber will immediately lead to failure of matrix and also the composite. In such a case the strength of unidirectional composite will exceed that of matrix.
14 What you learnt in this lecture? Mt Material ilaxes of a lamina, and the notion of transverse isotropy How to calculate density of a composite, using volume and mass fraction values. The rationale underlying development of predictive methodologies for estimating composite material properties Relations to predict longitudinal modulus of a unidirectional lamina Relations to predict strength of unidirectional lamina Different failure criterion for a unidirectional lamina which undergoes pure uniform tension
15 Rf References 1. Analysis and Performance of Fiber Composites, Agarwal, B.D.and Broutman, L. J., John Wiley & Sons. 2. Mechanics of Composite Materials, Jones, R. M., Mc Graw Hill. 3. Engineering Mechanics of Composite Materials, Daniel, I. M. and Ishai, O., Oxford University Press.
Materials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationANSYS Mechanical Basic Structural Nonlinearities
Lecture 4 Rate Independent Plasticity ANSYS Mechanical Basic Structural Nonlinearities 1 Chapter Overview The following will be covered in this Chapter: A. Background Elasticity/Plasticity B. Yield Criteria
More information1.050 Content overview Engineering Mechanics I Content overview. Selection of boundary conditions: Euler buckling.
.050 Content overview.050 Engineering Mechanics I Lecture 34 How things fail and how to avoid it Additional notes energy approach I. Dimensional analysis. On monsters, mice and mushrooms Lectures 3. Similarity
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationMATERIALS. Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle?
MATERIALS Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: A. Composition
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationFCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering
FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationLecture 7, Foams, 3.054
Lecture 7, Foams, 3.054 Opencell foams StressStrain curve: deformation and failure mechanisms Compression  3 regimes  linear elastic  bending  stress plateau  cell collapse by buckling yielding
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationIMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS OBTAINED WITH LMS SAMTECH SAMCEF
V ECCOMAS Thematic Conference on the Mechanical Response of Composites COMPOSITES 015 S.R. Hallett and J.J.C. Remmers (Editors) IMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS
More informationFlexure: Behavior and Nominal Strength of Beam Sections
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kipin.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationPLATE GIRDERS II. Load. Web plate Welds A Longitudinal elevation. Fig. 1 A typical Plate Girder
16 PLATE GIRDERS II 1.0 INTRODUCTION This chapter describes the current practice for the design of plate girders adopting meaningful simplifications of the equations derived in the chapter on Plate Girders
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationFiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens
Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: www.astm.org FiniteElement
More informationTesting and Analysis
Testing and Analysis Testing Elastomers for Hyperelastic Material Models in Finite Element Analysis 2.6 2.4 2.2 2.0 1.8 1.6 1.4 Biaxial Extension Simple Tension Figure 1, A Typical Final Data Set for Input
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More information4. SHAFTS. A shaft is an element used to transmit power and torque, and it can support
4. SHAFTS A shaft is an element used to transmit power and torque, and it can support reverse bending (fatigue). Most shafts have circular cross sections, either solid or tubular. The difference between
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationMECHANICAL PROPERTIES OF SOLIDS
Chapter Nine MECHANICAL PROPERTIES OF SOLIDS MCQ I 9.1 Modulus of rigidity of ideal liquids is (a) infinity. (b) zero. (c) unity. (d) some finite small nonzero constant value. 9. The maximum load a wire
More informationDelamination in the scoring and folding of paperboard
PEERREVIEWED CONVERTING Delamination in the scoring and folding of paperboard DOEUNG D. CHOI, SERGIY A. LAVRYKOV, and BANDARU V. RAMARAO ABSTRACT: Delamination between layers occurs during the creasing
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationThe Frictional Regime
The Frictional Regime Processes in Structural Geology & Tectonics Ben van der Pluijm WW Norton+Authors, unless noted otherwise 1/25/2016 10:08 AM We Discuss The Frictional Regime Processes of Brittle Deformation
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationBUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION
2 th International Conference on Composite Materials Copenhagen, 1924 th July 215 BUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION José Humberto S. Almeida Jr.
More information3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture,
3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it
More informationBrittle Deformation. Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm
Lecture 6 Brittle Deformation Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm WW Norton, unless noted otherwise Brittle deformation EarthStructure (2 nd
More informationTHEME IS FIRST OCCURANCE OF YIELDING THE LIMIT?
CIE309 : PLASTICITY THEME IS FIRST OCCURANCE OF YIELDING THE LIMIT? M M  N N + + σ = σ = + f f BENDING EXTENSION Ir J.W. Welleman page nr 0 kn Normal conditions during the life time WHAT HAPPENS DUE TO
More informationMechanical Design in Optical Engineering
OPTI Buckling Buckling and Stability: As we learned in the previous lectures, structures may fail in a variety of ways, depending on the materials, load and support conditions. We had two primary concerns:
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationDEFORMATION CAPACITY OF OLDER RC SHEAR WALLS: EXPERIMENTAL ASSESSMENT AND COMPARISON WITH EUROCODE 8  PART 3 PROVISIONS
DEFORMATION CAPACITY OF OLDER RC SHEAR WALLS: EXPERIMENTAL ASSESSMENT AND COMPARISON WITH EUROCODE 8  PART 3 PROVISIONS Konstantinos CHRISTIDIS 1, Emmanouil VOUGIOUKAS 2 and Konstantinos TREZOS 3 ABSTRACT
More informationA STUDY ON FATIGUE CRACK GROWTH IN CONCRETE IN THE PREPARIS REGION
VIII International Conference on Fracture Mechanics of Concrete and Concrete Structures FraMCoS8 J.G.M. Van Mier, G. Ruiz, C. Andrade, R.C. Yu and X.X. Zhang (Eds) A STUDY ON FATIGUE CRACK GROWTH IN CONCRETE
More informationCAPACITY DESIGN FOR TALL BUILDINGS WITH MIXED SYSTEM
13 th World Conference on Earthquake Engineering Vancouver, B.C., Canada August 16, 24 Paper No. 2367 CAPACITY DESIGN FOR TALL BUILDINGS WITH MIXED SYSTEM M.UMA MAHESHWARI 1 and A.R.SANTHAKUMAR 2 SUMMARY
More informationACET 406 MidTerm Exam B
ACET 406 MidTerm Exam B SUBJECT: ACET 406, INSTRUCTOR: Dr Antonis Michael, DATE: 24/11/09 INSTRUCTIONS You are required to answer all of the following questions within the specified time (90 minutes).you
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationPredicting Fatigue Life with ANSYS Workbench
Predicting Fatigue Life with ANSYS Workbench How To Design Products That Meet Their Intended Design Life Requirements Raymond L. Browell, P. E. Product Manager New Technologies ANSYS, Inc. Al Hancq Development
More informationGame Physics. Game and Media Technology Master Program  Utrecht University. Dr. Nicolas Pronost
Game and Media Technology Master Program  Utrecht University Dr. Nicolas Pronost Soft body physics Soft bodies In reality, objects are not purely rigid for some it is a good approximation but if you hit
More informationDon Robbins, Andrew Morrison, Rick Dalgarno Autodesk, Inc., Laramie, Wyoming. Abstract
PROGRESSIVE FAILURE SIMULATION OF ASMANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
More informationTask 1  Material Testing of Bionax Pipe and Joints
Task 1  Material Testing of Bionax Pipe and Joints Submitted to: Jeff Phillips Western Regional Engineer IPEX Management, Inc. 20460 Duncan Way Langley, BC, Canada V3A 7A3 Ph: 6045348631 Fax: 6045347616
More informationDerivation of minimum steel ratio: based on service applied stresses
MATEC Web of Conferences, () DOI:./ matecconf/ Derivation of minimum steel ratio: based on service applied stresses Humam AL Sebai,*, Salah Al Toubat University of Sharjah, Sharjah city, UAE Abstract.
More informationDegree Thesis Flexural Rigidity (D) in Beams. Author: Zious Karis. Instructor: Rene Herrmann
Degree Thesis Flexural Rigidity (D) in Beams Author: Zious Karis Instructor: Rene Herrmann Degree Thesis Materials Processing Technology 2017 DEGREE THESIS Arcada University of Applied Sciences, Helsinki,
More informationUSING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE
Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and
More informationJob No. Sheet 1 of 6 Rev B. Made by IR Date Oct Checked by FH/NB Date Oct Revised by MEB Date April 2006
Job No. Sheet 1 of 6 Rev B, Route de Limours Tel : (0)1 0 85 5 00 Fax : (0)1 0 5 75 8 Revised by MEB Date April 006 DESIGN EXAMPLE 6 BOLTED JOINT A 0 0 angle loaded in tension is to be connected to a gusset
More informationLecture 2: Deformation in the crust and the mantle. Read KK&V chapter 2.10
Lecture 2: Deformation in the crust and the mantle Read KK&V chapter 2.10 Tectonic plates What are the structure and composi1on of tectonic plates? Crust, mantle, and lithosphere Crust relatively light
More informationEE C245 ME C218 Introduction to MEMS Design
EE C245 ME C218 Introduction to MEMS Design Fall 2007 Prof. Clark T.C. Nguyen Dept. of Electrical Engineering & Computer Sciences University of California at Berkeley Berkeley, CA 94720 Lecture 16: Energy
More informationConstitutive models: Incremental plasticity Drücker s postulate
Constitutive models: Incremental plasticity Drücker s postulate if consistency condition associated plastic law, associated plasticity  plastic flow law associated with the limit (loading) surface Prager
More informationConcrete Technology Prof. B. Bhattacharjee Department of Civil Engineering Indian Institute of Technology, Delhi
Concrete Technology Prof. B. Bhattacharjee Department of Civil Engineering Indian Institute of Technology, Delhi Lecture  25 Strength of Concrete: Factors Affecting Test Results Welcome to module 6, lecture
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationDynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models
Dynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models I. Rhee, K.J. Willam, B.P. Shing, University of Colorado at Boulder ABSTRACT: This paper examines the global
More informationCivil Engineering Design (1) Design of Reinforced Concrete Columns 2006/7
Civil Engineering Design (1) Design of Reinforced Concrete Columns 2006/7 Dr. Colin Caprani, Chartered Engineer 1 Contents 1. Introduction... 3 1.1 Background... 3 1.2 Failure Modes... 5 1.3 Design Aspects...
More informationWrinkling Analysis of A Kapton Square Membrane under Tensile Loading
44th AIAA/ASME/ASCE/AHS Structures, Structural Dynamics, and Materials Confere 710 April 2003, Norfolk, Virginia AIAA 20031985 Wrinkling Analysis of A Kapton Square Membrane under Tensile Loading Xiaofeng
More informationME111 Instructor: Peter Pinsky Class #21 November 13, 2000
Toda s Topics ME Instructor: Peter Pinsk Class # November,. Consider two designs of a lug wrench for an automobile: (a) single ended, (b) double ended. The distance between points A and B is in. and the
More informationCRACK FORMATION AND CRACK PROPAGATION INTO THE COMPRESSION ZONE ON REINFORCED CONCRETE BEAM STRUCTURES
S. Kakay et al. Int. J. Comp. Meth. and Exp. Meas. Vol. 5 No. (017) 116 14 CRACK FORMATION AND CRACK PROPAGATION INTO THE COMPRESSION ZONE ON REINFORCED CONCRETE BEAM STRUCTURES SAMDAR KAKAY DANIEL BÅRDSEN
More informationOnedimensional ratchetting Twodimensional ratchetting Response of unified models Response of 2M1C model Response of polycrystalline models
Ratchetting Onedimensional ratchetting Twodimensional ratchetting Response of unified models Response of 2M1C model Response of polycrystalline models Still an open problem Ratchetting effects Primary
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More information6.37 Determine the modulus of resilience for each of the following alloys:
6.37 Determine the modulus of resilience for each of the following alloys: Yield Strength Material MPa psi Steel alloy 550 80,000 Brass alloy 350 50,750 Aluminum alloy 50 36,50 Titanium alloy 800 116,000
More informationArberi Ferraj. Wentworth Institute of Technology. Design of Machine Elements MECH 420
P a g e 1 Arberi Ferraj Wentworth Institute of Technology Design of Machine Elements MECH 420 P a g e 2 1. Executive Summary A scissor car jack was designed and must be reverseengineered in order to discover
More informationTINIUS OLSEN Testing Machine Co., Inc.
Interpretation of StressStrain Curves and Mechanical Properties of Materials Tinius Olsen has prepared this general introduction to the interpretation of stressstrain curves for the benefit of those
More informationAnalysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements
Acta Mech. Sin. (2016) 32(2):295 300 DOI 10.1007/s1040901505342 RESEARCH PAPER Analysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements V. H. Carneiro 1
More informationChapter 5. Vibration Analysis. Workbench  Mechanical Introduction ANSYS, Inc. Proprietary 2009 ANSYS, Inc. All rights reserved.
Workbench  Mechanical Introduction 12.0 Chapter 5 Vibration Analysis 51 Chapter Overview In this chapter, performing free vibration analyses in Simulation will be covered. In Simulation, performing a
More informationLecture #10: Anisotropic plasticity Crashworthiness Basics of shell elements
Lecture #10: 1510735: Dynamic behavior of materials and structures Anisotropic plasticity Crashworthiness Basics of shell elements by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering,
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationFundamentals of Durability. Unrestricted Siemens AG 2013 All rights reserved. Siemens PLM Software
Fundamentals of Durability Page 1 Your single provider of solutions System simulation solutions 3D simulation solutions Testbased engineering solutions Engineering services  Deployment services Troubleshooting
More informationMECHANICS OF MATERIALS
00 The McGrawHill Companies, Inc. All rights reserved. T Edition CHAPTER MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Teas Tech Universit
More information